Efficient free exciton emission at room temperature in Zn0.5Cd0.5Se/MgxZnyCd1KxKySe quantum wells
Efﬁcient free exciton emission at room temperature inZn0.5Cd0.5Se/MgxZnyCd1KxKySe quantum wellsO. Maksimova,*, N. Samartha, H. Lub, Martin Mun˜ozc, M.C. TamargobaDepartment of Physics, Pennsylvania State University, 104 Davey Lab, University Park, PA 16802, USAbDepartment of Chemistry, City College of New York, New York, NY 10031, USAcDepartment of Physics, Virginia Commonwealth University, Richmond, VA 23284, USAReceived 17 June 2004; received in revised form 7 July 2004; accepted 12 July 2004 by E.L. IvchenkoAvailable online 28 July 2004AbstractWe use temperature and power-dependent photoluminescence spectroscopy to demonstrate efﬁcient free exciton emission atroom temperature in high quality, strongly conﬁning Zn0.5Cd0.5Se/MgxZnyCd1KxKySe quantum wells. Our measurementsindicate that at low temperatures (T!50 K), the luminescence is dominated by bound exciton emission. However, free excitonemission becomes dominant at high temperatures (TO100 K) and persists up to room temperature with an intensity that isw40% that at cryogenic temperatures. We attribute these observations to the deep conﬁnement potential that stabilizes excitonsand prevents their thermal escape.q 2004 Elsevier Ltd. All rights reserved.PACS: 71.35.Cc; 71.55.Gs; 78.55.EtKeywords: A. ZnCdSe; B. Molecular beam epitaxy; E. PhotoluminescenceAlthough substantial success has been achieved in thedevelopment of AlxInyGa1KxKyN-based blue laser diodes(LDs), it is more challenging to produce long-lived devicesoperating in the green-yellow region (530–590 nm) due tothe high threshold current density required for lasing .Since AlxGayIn1KxKyP-based LDs operate at wavelengthslonger than 600 nm, this leaves an uncharted green–yellowspectral gap that is directly relevant for emerging technol-ogies such as the use of plastic optical ﬁbers that requiregreen lasers to achieve the lowest attenuation coefﬁcient.Together with improvements in the degradation stability,this revives interest in ZnxCd1KxSe-based lasers that cancover this part of the spectrum . A large effort has beendevoted to the development of emitters with a quantum dot(QD) active layer and QD-based LDs have been demon-strated . However, their performance is limited to wellbelow room temperature by the thermal escape of excitonsfrom conﬁned states towards non-radiative recombinationchannels .In this letter, we report the observation of efﬁcient freeexciton (FE) luminescence at room temperature in stronglyconﬁning Zn0.5Cd0.5Se/MgxZnyCd1KxKySe quantum wells(QWs). We demonstrate that the conﬁnement of excitons indeep and narrow QWs (dQWw3 nm or 10 ml) both stabilizesFEs and prevents their escape to the barriers, resulting inefﬁcient radiative recombination at room temperature.Further, the high quality of these lattice-matched structuresreduces the inﬂuence of non-radiative centers. Both thesefactors counteract the usual mechanisms that quenchluminescence with increasing temperature, leading to FEemission at room temperature with an intensity that isw40% of the emission intensity at low temperatures.QW structures are grown by molecular beam epitaxy0038-1098/$ - see front matter q 2004 Elsevier Ltd. All rights reserved.doi:10.1016/j.ssc.2004.07.022Solid State Communications 132 (2004) 1–5www.elsevier.com/locate/ssc* Corresponding author. Tel.: C1-814-863-9514; fax: C1-814-865-3604.E-mail address: email@example.com (O. Maksimov).
(MBE) on (001) InP substrates, as described elsewhere .They consist of a lattice matched In0.5Ga0.5As buffer layer,MgxZnyCd1KxKySe barrier layers (xw0.5, Egz3.0 eV), anda Zn0.5Cd0.5Se (Egz2.18 eV) well layer. The thickness ofthe bottom and the top barriers are 500 and 100 nm,respectively. QWs are characterized by photoluminescence(PL) and electroreﬂectance spectroscopies. PL measure-ments are performed in a liquid He continuous ﬂow cryostatin a temperature range from 10 to 300 K. The 404-nm line ofa LD is used for the excitation. The PL is collected in a back-scattering geometry, spectrally resolved by a monochroma-tor and detected by a cooled charge coupled device arraydetector. Electroreﬂectance measurements are performed atroom temperature as described elsewhere .Fig. 1 shows the PL spectrum at 10 K of a structure witha 3 nm wide well. (The 10 K PL spectra of structures withslightly different well widths are shown in the inset.) Thebarrier emission is at 2.978 eV and the QW emission is at2.312 eV. The QW emission is signiﬁcantly stronger thanthe barrier emission, suggesting that the majority of photo-excited carriers are captured by the QW prior to recombina-tion. The absence of deep level emission is indicative ofhigh crystalline quality. Since most of the band disconti-nuity in the MgxZnyCd1KxKySe/Zn0.5Cd0.5Se system is inthe conduction band (DEC/DEgw0.8) , the conductionand valence band offsets are 533 and 133 meV, respectively.This is larger than for ZnxCd1KxSe/ZnSySe1Ky QWs [7,8]and signiﬁcantly exceeds the thermal activation energyproviding sufﬁcient quantum conﬁnement even at roomtemperature (kBTZ25 meV).Fig. 2 shows PL spectra of a 3 nm thick QW taken atdifferent temperatures. The 10 K PL spectrum is dominatedby a single spectral peak (A) that has an asymmetric lineshape with a low energy tail. A higher energy peak B (DEZ22 meV) emerges at w30 K. As the temperature increases,both peaks red shift and the intensity of A decreases, whilethat of B increases. Finally, A disappears above 100 K whileB persists up to room temperature and exhibits a gradual redshift, accompanied by a decrease in intensity and an increasein linewidth.Fig. 3 shows room temperature electroreﬂectance (dottedline) and PL (solid line) spectra for comparison. The energyof the PL emission corresponds to the electron-heavy holeexcitonic transition suggesting the free excitonic (FE) originof luminescence. Based upon its position and temperaturedependence, the higher energy peak (B) is assigned to a FE.The lower energy peak (A) can be attributed to a boundexciton (BE), biexciton, or charged exciton. To identify itsorigin, we study the dependence of the peak emissionintensity on the excitation laser density at 10, 60, 100 and300 K. Superlinear behavior is not observed indicating theFig. 1. Photoluminescence (PL) spectrum of a Zn0.5Cd0.5Se/Mgx-ZnyCd1KxKySe quantum well (QW) structure with a 3 nm thick welllayer taken at 10 K. The inset of the ﬁgure shows 10 K PL spectra ofQW structures with different well thickness.Fig. 2. Photoluminescence spectra of a 3 nm thick Zn0.5Cd0.5-Se/MgxZnyCd1KxKySe QW taken at different temperatures. Thesolid lines correspond to the spectra while the dotted lines areGaussian ﬁts.O. Maksimov et al. / Solid State Communications 132 (2004) 1–52
absence of biexcitons or charged excitons. Instead, we ﬁndthat the intensity of both peaks A and B increases linearlywith excitation laser density and a slope (k) near unity isobtained over the whole temperature range (Table 1). Thisshows the excitonic origin of the emission  that persistsup to room temperature.To elucidate whether a BE contributes to the QWluminescence, we plot the integrated PL intensity for A andB as a function of temperature in Fig. 4. For convenienceand to avoid the use of absolute intensities (A), theintegrated intensity (I) is deﬁned as:IJðTÞ Z AJðTÞ=ðAAðTÞ CABðTÞÞ J Z A; B (1)The emission intensity is proportional to both thepopulation density of excitons (Nj) and recombinationefﬁciency (nj):AJ Z njNj (2)The nj is expressed as a function of radiative (tR) andnon-radiative (tNR) recombination times :nj Z ð1 CtR=tNRÞK1(3)Since BEs are thermally activated to FEs, the Nj can bedescribed as w[1Kexp(KDE/kBT)] for BEs and w[0Cexp(KDE/kBT)] for FEs, where DE is the energy bindingexciton to localization center. If we assume that recombina-tion efﬁciency does not change with temperature and neglectother level depopulation mechanisms, we can write theintegrated intensity of BE and FE lines as:IBE Z nBE ð1 KexpðKDE=kBTÞ=½nBEð1 KexpðKDE=kBTÞCnFE expðKDE=kBTÞ ð4ÞIFE Z nFE expðKDE=kBTÞ=½nBEð1 KexpðKDE=kBTÞCnFE expðKDE=kBTÞ (5)The ﬁt based on this simpliﬁed model is shown withdotted lines in Fig. 4. It follows the experimental data andjustiﬁes the assignment of B to FE emission and A to BEemission. The recombination efﬁciency for FEs, estimatedfrom the ﬁt, is higher than the BE recombination efﬁciency(nFE/nBEZ7.7). This is in agreement with the observationthat FEs have a shorter radiative recombination time thanBEs . The gap between BE and FE lines (DE) decreaseswith increasing QW thickness, from 24 meV for a 2.85 nmthick well to 20 meV for a 4.3 nm thick well, as shown inTable 1. The origin of the BE emission is unclear and can beexplained by different mechanisms. First, since the wellthickness is smaller than the exciton Bohr radius(a0w4.9 nm) , while the conﬁnement potential isFig. 3. Room temperature photoluminescence (solid line) andelectroreﬂectance (dotted line) spectra of a 3 nm thick Zn0.5Cd0.5-Se/MgxZnyCd1KxKySe QW.Table 1Properties of the Zn0.5Cd0.5Se/MgxZnyCd1KxKySe quantum well structuresdQW (nm) k at 10 K k at 60 K k at 300 K PL Inten-sity at 10 K(arb. units)PL Inten-sity at100 K (arb.units)PL Inten-sity at300 K (arb.units)DE (meV) E0B (Cl0X)(meV)E2D(meV)2.85 1.05 1.08 1.18 1 1.30 0.95 24 22.0 42.93 1.06 1.11 1.18 1 0.78 0.23 22 21.7 42.24.3 1.05 1.06 1.22 1 1.02 0.4 20 19.0 37.0Fig. 4. Dependence of the integrated intensity of bound exciton(solid circles) and free exciton (open circles) emission lines as afunction of temperature for a 3 nm thick Zn0.5Cd0.5Se/MgxZnyCd1KxKySe QW. The dotted lines are the ﬁts.O. Maksimov et al. / Solid State Communications 132 (2004) 1–5 3
large, roughness of the well/barrier interface and/or alloydisorder in the barrier layers can provide signiﬁcantly deeplocalization states. Second, composition ﬂuctuations inZn0.5Cd0.5Se alloy forming the well can cause excitonlocalization in the regions with increased cadmium content[13,14]. However, since Zn0.5Cd0.5Se/MgxZnyCd1KxKySeQWs are lattice matched in contrast to compressivelystrained ZnxCd1KxSe/ZnSe QWs, the formation of cad-mium-rich regions is unlikely. Finally, donor and/oracceptor bound excitons can contribute to the emission.ZnCl2 cell is installed in MBE system and routinely used forn-type doping. Thus, due to the background doping,recombination of neutral donor bound excitons (Cl0X) islikely to contribute at low temperatures. The Cl0X bindingenergy ðE0BÞ is w9 meV in ZnSe . Quantum conﬁnementwill increase ðE0BÞ to 20–22 meV, as shown in Table 1. Theestimated values are close to DE, indicating that Cl0Xrecombination is a possible origin of the BE line.The intensity of the QW emission is shown as anArrhenius plot in Fig. 5. All QWs exhibit strong roomtemperature luminescence, comparable to that at 10 K. Theyalso exhibit a non-monotonic dependence of the intensity ontemperature. This temperature dependence is anomalous forZnxCd1KxSe QWs [7,8,16], but can be explained by a BE toFE transition. At low temperatures, where the BE emissiondominates the decrease in emission intensity with increasingtemperature is caused by thermal excitation of BEs to FEs.Over the temperature range 75–125 K, the increase inemission intensity is due to the higher FE recombinationefﬁciency. At the highest temperatures studied, the decreasein intensity is caused by exciton dissociation, exciton escapefrom the well to the barriers, and/or the transfer to the non-radiative recombination centers. However, the decrease issmall and the room temperature emission intensity is stillw40% of that at 100 K, as shown in Table 1. We believethis is due to the suppression of the mechanisms mentionedabove.We now estimate the increase in exciton binding energydue to the QW conﬁnement using the results of a provenanalytical technique . For an inﬁnitely deep QW, theexciton binding energy (E2D) can be written as:E2DZ E3D=f½1 Cða K3Þ=2g2; (6)where E3Dis the exciton binding energy in the bulk, and a isa dimensionless parameter that varies with the quantum wellwidth dQW as follows:a Z 3 KexpðKdQW=2a0Þ: (7)For a ﬁnite conﬁnement potential, where wave functiondecay into the barrier decreases conﬁnement, the aboveresults are modiﬁed by deﬁning an effective length scaled*QW  as:d*QW Z ð2=jBÞ CdQW (8)where 1=jB Z1=jBE C1=jBH; jBE and jBH are the wave vectorsolutions of the transcendental equations that result fromsolving the relevant Schro¨dinger equations for electrons andholes in the QW potential. The results of our calculations(Table 1) show that the exciton binding energy increasesfrom the bulk value of 17.5 meV  to w40 meV,preventing exciton dissociation even at room temperature.We next use a semi-empirical model to estimate thecarrier loss due to the thermally activated escape from thewell (h) :h Z 1 K2=ð2 C100T expðKE=kBTÞÞ (9)where T is the temperature and E is the conﬁnement energy.A 350 meV conﬁnement limits carrier loss to 1% at roomtemperature. In our case conﬁnement energy exceeds650 meV and thermal escape is negligible.Finally, we address the issue of transfer to non-radiativerecombination centers, which is well known to signiﬁcantlydecrease room temperature luminescence. For instance, inmaterial systems such as InxGa1KxN with large misﬁtdislocation densities, this mechanism results in a rapid dropof emission intensity in InxGa1KxN QWs (TO150 K) and degrades room temperature performance of InxGa1KxNLEDs (defect density w109cmK2) . Since MgxZny-Cd1KxKySe heterostructures are lattice matched and thedefect density is small (!105cmK2) , we do not expectthis mechanism to be efﬁcient.In conclusion, Zn0.5Cd0.5Se/MgxZnyCd1KxKySe QWsare characterized by PL spectroscopy. BE emissiondominates below 50 K, while FE emission dominatesFig. 5. Arrhenius plot of the emission intensity versus inversetemperature.O. Maksimov et al. / Solid State Communications 132 (2004) 1–54
above 100 K and persists up to room temperature. The roomtemperature emission is strong and comparable to the lowtemperature emission due to the efﬁcient quantum conﬁne-ment that suppresses non-radiative recombination mechan-isms. This indicates high quantum efﬁciency and suggeststhat Zn0.5Cd0.5Se/MgxZnyCd1KxKySe QWs are attractivefor application as lasers, operating in green spectral range.Finally, we note that these excitonic light emitters may alsoplay an important role in the development of triggered singlephoton sources that function at elevated temperatures .AcknowledgementsM.M., H.L., and M.C.T. were supported by NSF throughgrant ECS0217646. O.M. and N.S. acknowledge the supportof the DARPA-QUIST program through the Center forSpintronics and Quantum Computation, University ofCalifornia-Santa Barbara.References S. Nakamura, M. Senoh, S. Nagahama, N. Matsushita,T. Mukai, Appl. Phys. Lett. 76 (2000) 22. S.V. Ivanov, Phys. Status Solidi A 192 (2002) 157. S.V. Ivanov, A.A. Toropov, S.V. Sorokin, T.V. Shubina,V. Sedova, A.A. Sitnikova, P.S. Kop’ev, Zh.I. Alferov,A.A. Waag, H.J. Lugauer, G. Reuscher, M. Keim,G. Landwehr, Appl. Phys. Lett. 74 (1999) 498. I.C. Robin, R. Andre, L.S. Dang, H. Mariette, S. Tatarenko,J.M. Gerard, K. Kheng, F. Tinjod, M. Bartels, K. Lischka,D. Schikora, Phys. Status Solidi B 241 (2004) 543. L. Zeng, S.P. Guo, Y.Y. Luo, W. Lin, M.C. Tamargo, H. Xing,S.G. Cargill III, J. Vac. Sci. Technol. B 17 (1999) 1255. M. Mun˜oz, H. Lu, X. Zhou, M.C. Tamargo, F.H. Pollak, Appl.Phys. Lett. 83 (2003) 1995. E. Oh, S.D. Lee, H.D. Jung, J.R. Kim, M.D. Kim, B.J. Kim,J.K. Li, H.S. Park, T.I. Kim, S.V. Ivanov, A.A. Toropov,T.V. Shubina, J. Appl. Phys. 80 (1996) 5951. I. Lo, K.H. Lee, L.W. Tu, J.K. Tsai, W.C. Mitchel, R.C. Tu,Y.K. Su, Solid State Commun. 120 (2001) 155. T. Schmidt, K. Lischka, W. Zulehner, Phys. Rev. B 42 (1992)8989. M. Sugarawa, Phys. Rev. B 51 (1995) 10743. L. Aigouy, V. Mathet, F. Liaci, B. Gil, O. Briot, T. Cloitre,M. Averous, L. Aloumbard, Phys. Rev. B 53 (1996) 4708. I. Hernandez-Calderon, in: M.C. Tamargo (Ed.), II–VISemiconductor Materials and Their Applications, Taylor andFranics, New York, 2002. S. Permogorov, A. Klochikhin, A. Reznitsky, J. Lumin. 100(2002) 243. S. Permogorov, A. Klochikhin, A. Reznitsky, L. Tenishev,S. Ivanov, S. Sorokin, C. Klingshirn, J. Cryst. Growth 214(2000) 1158. S.Z. Wang, S.F. Yoon, L. He, X.C. Shen, J. Appl. Phys. 90(2001) 2314. C. Morhain, G.D. Brownlie, E. Tournie, A. Masi,C. Ongaretto, K.A. Prior, J.P. Faurie, B.C. Cavenett,J. Cryst. Growth 184 (1998) 591. H. Mathieu, P. Lefebrve, P. Christol, J. Appl. Phys. 72 (1992)300. J. Camacho, I. Loa, A. Cantarero, I. Hernandez-Calderon,Microelectron. J. 33 (2002) 349. N. Grandjean, B. Damilano, J. Massies, S. Dalmasso, SolidState Commun. 113 (2000) 495. T. Stephan, M. Kunzer, P. Schlotter, W. Pletschen, H. Obloh,S. Mu¨ller, K. Ko¨hler, J. Wagner, Phys. Status Solidi A 194(2002) 568. K. Sebald, P. Michler, T. Passow, D. Hommel, G. Bacher,A. Forchel, Appl. Phys. Lett. 81 (2002) 2920.O. Maksimov et al. / Solid State Communications 132 (2004) 1–5 5